_{1}

^{*}

Production of axisymmetric pieces by technology of sheet metal drawing is widespread nowadays. So the calculation analysis of capacity and forces necessary for deformation is of special interest. The length of cylindrical pieces with axisymmetric deformation is limited by loss of stability and buckling due to the development of side strains. A new technological process is based on making considerable number of folds—18 - 26 with the amplitude of 0.8 - 0.9 mm— before the deformation or immediately after the partial one. That reduces the stiffness of billets and prevents from development of large size buckles. A new technological process is developed for producing a long run of high-quality products.

Axisymmetric deformation of sheet metal blanks are widely used in the manufacture of cylindrical pieces made of flat metal sheets.

Such products as various vessel bodies, nozzles, connecting pipes are made of low carbon steels as well as of copper, brass, magnesium alloys and other metals.

This paper examines only the deformation of the products with axial symmetry, which are increasingly used in industry.

Regularities of plastic deformation are studied in research papers [1-4]. They demonstrate that under the pressure of a cylindrical die on the center of the workpiece which was initially shaped like a disk, the plane stress is developed, with only two of the six tensor components being nonzero. Due to tensile radial stress and compressive tangential stress [1,2] the buckling of deformable workpiece accompanied with folds is possible. Usually this leads to waste metal and therefore it is necessary to limit the length of a product, to use drawing with subsequent additional deformation (secondary drawing operation, rolling).

To prevent the occurrence of folds the blank holders are used, but this significantly increases the deformation strain to an extent of the occasional overdrawing occurrence in a deformable work piece. Sometimes drawing with the billet or its edge parts heating (near the maximum diameter) is used. For some metals billet heating can increase the allowed length of a product by 1.5 - 2.0 times.

Magnesium alloy sheets are thought to be used for deep drawing only with the billet heating. But as the thickness of a sheet metal to be deformed is small (up to 1 - 3 mm) and is exposed to chilling it has to be heated directly on a die. That complicates the design of the equipment, enhances significantly power consumption and makes it difficult to ensure safety conditions.

In this paper we discuss some features of the sheet blanks axsymmetric strain. A new drawing technique which allows to improve the technology and to expand significantly the range of products is proposed and investigated.

The graphic pattern of drawing deformation is illustrated in _{0} and inner one R_{1}, thickness h and punch 3 which moves along axis Z with constant velocity V_{z} = ‒V_{0}.

Kinematically admissible velocity field determines the upper limit of deformation ca capacity N and the associated moving die force P. Such a velocity field is to satisfy: a) the incompressibility condition, b) velocity boundary conditions, c) the condition under which the deformation capacity is positive [_{1} moves with velocity V_{z}_{ }= ‒V_{0} together with moving die 3 [2,3]. In this zone V_{r} is equal to 0 (the coordinate axes location is shown in _{1} + h and r = R_{0}. Some features of this deformation are considered in paper [

with the strain-rate tensor components

(the other tensor components are equal to zero). Value is velocity under and the second invariant of strain-rate tensor is equal to

This velocity field can be assumed as kinematically admissible only if there exists surface z(r) separating the two selected deformation zones. On this surface the normal rate components are to be equal, (tangential components may differ and their difference determines the capacity of the shear). Such a surface exists and is a paraboloid [

where is yield point in shear, and shear capacity over the surface of paraboloid is

with paraboloid equation:

tangential components break at the boundary of two zones

with shear capacity

Full capacity with provision for friction load at the surface of lower die is

where is coefficient of sliding friction. Moving die force is

If the deformation is carried out with the use of blankholder, with force T, the friction load increases and force P is equal to

Usually and the force is

If the steel sheet deformation is carried out without the use of blankholder, as shown in

, ,; h = 1 mm, m = 0.10, ,), the value of force according to (5) is P= 0.13 MN.

As usual, the kinematically admissible velocity field determines the upper limit of forces (i.e., overstated values of P). According to experimental data, in case of drawing this overstatement amounts to 20% - 25%. This is acceptable for the choice of equipment in most cases.

In the process of deep drawing a sheet shaped initially like a disk undergoes tangential compressive stress that can lead to loss of stability. Thereby folds occur on the part of a surface, as shown in

Usually, the fold occurrence, i.e. wavy surface with amplitude of up to 10 - 20 mm, leads to inability to output products and to rejected material. From Saint-Venan condition end equation of equilibrium

and condition of plasticity

it is clear that stress is

where the integration constant is determined by the condition of with Tangential stress with is equal to.

The minimum allowable value, (under which folds occur) is determined by parameters:, h, Е_{Т}_{ } with the dimensions: m (for the first three) и МН/m^{2} for yield limit and plastic deformation hardening modulus. Here is a value characterizing metal hardening in plastic deformation.

Out of these five variables it is possible to form three dimensionless parameters:

and

As well as to determine approximately strain-hardening characteristic, where is ultimate strength.

According to theorem the relationship between the above-mentioned parameters must take the following form . Having solved it for, we get

Based on the data of many deformation experiments with carbon steel sheets of 0.5 mm, 1.00 mm, 1.5 mm and 2.0 mm thicknesses the graphs were plotted as given on

The relationship (8) can be determined with the empirical formula for a maximum permissible (minimum) value

To provide the sheet stability the following condition should be fulfilled:

Since the maximum possible upset length is equal to

it follows from (9) that the maximum possible length of work is

For example, for a steel sheet of h = 1 mm thickness

with, , ; . according to Formula (9) we get,; l = 8.6 mm.

Formula (9) can be applied if and the experimental data spread is considerable which is seen from

It conforms to the test which shows what should be applied for metal (alloys) drawing with high hardening: the higher is, the easier the deformation can be made, and the larger work length can be produced when drawing. Metals with minor hardening with graph of function being close to a perfectly plastic body graph (i.е. when ) are unfit for deep drawing.

Steel sheets with up to 0.05% - 0.15% temper and not more than 20 - 30 µm grain size with extension strain of no less than 40% are often used fro drawing.

According to the above-mentioned the holder allows to increase l value and decrease parameter . However, the ring crack wastage increases as shown on

Based on the research conducted a new technological drawing process has been suggested (see Patent Application of Russian Federation №2011123174/02, MPK 7В1D 22/02 from 08 June 2011).

The method consists in forming a series of waves (ridges) along a ring on a disk-form billet, see

Experiments were made with samples of diameters 70 - 120 mm and height 80 - 140 mm of low carbon steels.

The waves may be located not along the billet edge as shown on

Various wave variants are also shown on Figures 5(c) and (d), e. The depth for 0.5 mm sheets of carbon steel was 0.5 mm, the number of waves being 18 - 26. “The loss of stability” with large wave formation, e.g. shown on

The deformation is sure to result in increasing the wave amplitude, sometimes 1.5 times (there occurs their compression with “wave” shortening sometimes in 2 - 3 times), but the new waves of large amplitude do not emerge (e.g. as those shown on

The main idea of the method consists in making a large number (18 - 26) of waves of small amplitude on a sheet (disk) in advance in order to avoid the potential of emerging 4 - 8 “waves” (buckles) of large amplitude (up to 10 - 20 mm). It decreases the rigidity of a deformed billet, with the amplitude being able to reach 1.5 mm after drawing, which does not lead to sharp changes of the whole product pattern (it usually happens with the stability loss) and allows to manufacture the required product of high quality.

These Filter Casing Blanks were made from low carbon steel (st.08 according Russian standart 1050 - 88). Quality of Carbon was 0.05% - 0.25%. Part of filter Casings was made of semi-killed steel (st.3). Diameters of these Casing Blanks were 96 mm and their height was 92 mm. Artificial waves were made with length 28 mm and amplitudes 1 mm. Quanlity of Filters was good and reject was decreased twice till 0.75%.

The artificial waves (ridges) are certain to remain on the product. The method is sure not to be used in cases when even small waves on the product cannot be allowed. But in many cases such waves with amplitude of less than 1mm do not at all make the product quality worse and therefore are possible. So the above-mentioned Tver plant manufactured more than 10 thousand filter casings (

it loses stability when being subject to compressive deformation, (where F is an area of bar section, J is its moment of inertia, l is a bar length).

With further compression a bar loses its configuration, with the deflection increasing rapidly up to 0.5 l and more.

If a bar can be manufactured as shown on

(Both the rings and deformable bodies of

In some cases the manufactured rigidity reduction of the billet being drawn can be rational.

The following conclusions can be deduced from the above-said study:

1) The axially symmetric sheet blank deformation under drawing has been examined.

The kinematically admissible velocity field for force upper limits has been built.

2) A new method of drawing which included making ridges-waves of small amplitude on a blank before drawing has been proposed and studied. But the number of such waves should be considerable and it gives the possibility to avoid the formation of more significant form distortions of a billet.

3) The method was used for producing oil filter casings and getting a high-quality product. More than 10 thousand filter casings of good qualities of carbon steel were produced with use of new method.